#------------------------------------------------------------------------------
#$Date: 2016-02-13 21:28:24 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176429 $
#$URL: svn://www.crystallography.net/cod/cif/1/10/12/1101209.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1101209
loop_
_publ_author_name
'Ouellette, Wayne'
'Yu, Ming Hui'
'O'Connor, Charles J.'
'Zubieta, Jon'
_publ_section_title
;
 Structural Diversity of the Oxovanadium Organodiphosphonate System:
 A Platform for the Design of Void Channels
;
_journal_issue                   8
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3224
_journal_page_last               3239
_journal_paper_doi               10.1021/ic0517422
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'C4.5 H12.75 N O9 P2 V2'
_chemical_formula_weight         388.73
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 103.5240(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   15.2345(10)
_cell_length_b                   10.1817(6)
_cell_length_c                   18.6968(12)
_cell_measurement_temperature    90(2)
_cell_volume                     2819.7(3)
_diffrn_ambient_temperature      90(2)
_exptl_crystal_density_diffrn    1.831
_cod_duplicate_entry             1101187
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_original_formula_sum        'C4.50 H12.75 N O9 P2 V2'
_cod_database_code               1101209
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
V1A V 0.75200(8) -0.04720(8) 0.21718(4) 0.0152(3) Uani 0.898(5) 1 d P . 1
O2 O 0.6543(2) 0.0084(3) 0.2165(2) 0.0351(9) Uani 0.898(5) 1 d P . 1
V1B V 0.8047(10) -0.0750(7) 0.2187(3) 0.027(4) Uani 0.102(5) 1 d P . 2
O2B O 0.9094(17) -0.123(3) 0.2292(16) 0.028(7) Uani 0.102(5) 1 d P . 2
V2 V 0.66193(4) 0.38449(5) 0.08390(3) 0.01656(16) Uani 1 1 d . . .
P1 P 0.66171(6) -0.33276(8) 0.16590(5) 0.0162(2) Uani 1 1 d . . .
P2 P 0.78554(7) 0.11826(8) 0.07647(5) 0.0169(2) Uani 1 1 d . . .
O1 O 0.73127(18) -0.2227(2) 0.17113(14) 0.0231(6) Uani 1 1 d . . .
O3 O 0.8302(2) 0.0982(2) 0.26029(13) 0.0242(6) Uani 1 1 d . . .
O4 O 0.78635(19) -0.0033(2) 0.12477(13) 0.0213(5) Uani 1 1 d . . .
O5 O 0.70163(18) 0.2009(2) 0.07478(14) 0.0205(5) Uani 1 1 d . . .
O6 O 0.7048(3) 0.3551(3) 0.19028(15) 0.0333(8) Uani 1 1 d . . .
O7 O 0.55530(19) 0.3646(3) 0.05936(17) 0.0299(6) Uani 1 1 d . . .
O8 O 0.67459(19) 0.5735(2) 0.10537(13) 0.0207(5) Uani 1 1 d . . .
O9 O 0.71048(19) 0.4320(3) -0.00036(13) 0.0227(6) Uani 1 1 d . . .
C1 C 0.5521(3) -0.2609(4) 0.1419(2) 0.0231(7) Uani 1 1 d . . .
N1 N 0.2641(9) 0.2766(12) 0.0180(7) 0.074(4) Uani 0.50 1 d PD . .
H1A H 0.5458 -0.2008 0.1820 0.028 Uiso 1 1 calc R . .
H1B H 0.5477 -0.2071 0.0971 0.028 Uiso 1 1 calc R . .
C2 C 0.4727(3) -0.3569(3) 0.1277(2) 0.0216(7) Uani 1 1 d . . .
H2A H 0.4769 -0.4136 0.1714 0.026 Uiso 1 1 calc R . .
H2B H 0.4755 -0.4139 0.0854 0.026 Uiso 1 1 calc R . .
C3 C 0.8826(3) 0.2173(3) 0.1114(2) 0.0203(7) Uani 1 1 d . . .
H3A H 0.8849 0.2876 0.0753 0.024 Uiso 1 1 calc R . .
H3B H 0.8755 0.2601 0.1573 0.024 Uiso 1 1 calc R . .
N2 N 0.4051(12) 0.2896(10) 0.1091(14) 0.176(12) Uani 0.50 1 d PD . .
C4 C 0.3468(10) 0.2035(15) 0.0188(9) 0.084(5) Uani 0.50 1 d PD . .
C5 C 0.4038(12) 0.1502(10) 0.0907(8) 0.087(5) Uani 0.50 1 d PD . .
C6 C 0.4889(11) 0.0788(13) 0.0812(11) 0.22(2) Uani 0.50 1 d PD . .
H6' H 0.715(4) 0.292(5) 0.195(3) 0.038(16) Uiso 1 1 d . . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
V1A O2 1.590(4) . ?
V1A O3 1.952(3) . ?
V1A O4 1.970(3) . ?
V1A O6 1.971(3) 4_645 ?
V1A O1 1.977(3) . ?
V1B O2B 1.630(3) . ?
V1B O4 1.862(6) . ?
V1B O6 1.881(7) 4_645 ?
V1B O3 1.930(7) . ?
V1B O1 1.959(8) . ?
V2 O7 1.594(3) . ?
V2 O9 1.951(3) . ?
V2 O6 1.966(3) . ?
V2 O8 1.966(2) . ?
V2 O5 1.984(3) . ?
P1 O8 1.528(2) 1_545 ?
P1 O3 1.528(3) 4_645 ?
P1 O1 1.529(3) . ?
P1 C1 1.782(4) . ?
P2 O5 1.525(3) . ?
P2 O9 1.526(3) 7_655 ?
P2 O4 1.530(3) . ?
P2 C3 1.783(4) . ?
O3 P1 1.528(3) 4_655 ?
O6 V1B 1.881(7) 4_655 ?
O6 V1A 1.971(3) 4_655 ?
O6 H6' 0.67(5) . ?
O8 P1 1.528(2) 1_565 ?
O9 P2 1.527(3) 7_655 ?
N1 C4 1.460(2) . ?
C1 C2 1.529(5) . ?
C1 H1A 0.9900 . ?
C1 H1B 0.9900 . ?
C2 C3 1.534(5) 3_445 ?
C2 H2A 0.9900 . ?
C2 H2B 0.9900 . ?
C3 C2 1.534(5) 3 ?
C3 H3A 0.9900 . ?
C3 H3B 0.9900 . ?
N2 C5 1.460(2) . ?
C5 C6 1.531(2) . ?
